bubble rupture in bubble...
Embed Size (px)
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149 1141
BUBBLE RUPTURE IN BUBBLE ELECTROSPINNING
Rouxi CHEN a,b, Yuqin WAN
d, Na SI c, Ji-Huan HE
a,b*, Frank KO d,
and Shu-Qiang WANG e*
a National Engineering Laboratory for Modern Silk, College of Textile and Clothing Engineering, Soochow University, Suzhou, China
b Nantong Textile Institute of Soochow University, Nantong, China c Nantong Bubbfil Nanotechnology Company Limited, Nantong, China
d Department of Material Engineering, University of British Colombia, Vancouver, Canada e Research Center for High Performance Computing, Shenzhen Institutes of Advanced Technology,
Chinese Academy of Sciences, Shenzhen, China
Review paper DOI: 10.2298/TSCI1504141C
As the distinctive properties and different applications of nanofibers, the demand of nanofibers increased sharply in recently years. Bubble electrospinning is one of the most effective and industrialized methods for nanofiber production. To op-timize the set-up of bubble electrospinning and improve its mass production, the dynamic properties of un-charged and charged bubbles are studied experimental-ly, the growth and rupture process of a bubble are also discussed in this paper. Key words: bubble electrospinning, bubbfil spinning, dynamic of bubble,
growth and rupture of bubble, nanofiber, mass production
Nanofibers have been extensively explored in last decades ; their distinctive properties (high surface area in combination with different functionalities) make them one of the most promising candidates in diverse areas , such as filter, tissue engineering, drug de-livery, protective clothing, advanced biomaterials, biosensors, etc.
Conventional single-needle electrospinning is a simple, effective, versatile, cost-effective method to produce polymer nanofibers. However, it has a small fiber production rate, typically less than 0.3 g per hour per needle , which greatly limits its practical applica-tions in industrial and civil products. Recently the needle-less (free liquid surface) electrospinning technology have been reported as new viable possibilities to fabricate nanofibers in mass production . Hundreds of labs and research institutions have attempted to find new methods to improve the production of nanofibers.
Bubble electrospinning is one of the most influential needle-less electrospinning methods, and it has been developed into a matured bubbfil spinning . Inspired by the fantas-tic spider spinning, Liu and He  and Liu et al.  used a gas pump to generate bubbles on a polymer liquid surface which was charged with an electric voltage, a number of jets were gen-erated from the surface of the bubbles. They also applied “theory of bubble dynamics” to ex-plain the mechanism of mass nanofiber production [8, 9]. In a number of publications, efforts have been described in finding the controlling parameters for different polymers using bubble –––––––––––––– * Corresponding authors; e-mails: [email protected], [email protected]
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning 1142 THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149
electrospinning. Yang et al.  investigated the effects of solution concentration and viscosity on the diameter and morphology of bubble electrospun polyvinyl alcohol (PVA) nanofibers. Kong et al.  suggested a new method for fabrication of nanofibers with a polymer bubble membrane, and studied the effects of applied voltage and collect distance on the fiber diameter. Gule et al.  used bubble electrospinning to prepare DMHF-containing PVA nanofibers, which demonstrated good antimicrobial and cell-adhesion inhibition efficiency. Dou et al.  investigated the morphology of nylon6/66 nanofibers yarns produced by bubble-spinning. Chen et al. fabricated crimped nanofibers by bubble electrospinning and explored its crimp mecha-nism . The authors also described the surface tension of a bubble with a modified Young-Laplace equation , which can be widely applied for bubble spinning process analysis. Li et al.  studied the effect of airflow direction blowing on polymer bubble and the morphology difference of the superfine fibers. Li et al.  compared the fiber morphologies of polyether sulfone (PES) via bubble spinning vs. conventional single needle electrospinning under the same spinning conditions. Shen et al.  prepared multi-layer nanofiber nonwoven fabrics for PM2.5 mask, which admitted excellent filter capabilities and breathability. Sidaravicius et al.  fabricated PEO/PVA nanofibers using a bubble foamed polymer solution to promote high mass deposition and investigate its deposited intensity. Ren et al.  used the foaming-assisted electrospinning technique to get large-pore mesoporous ZnO nanofibers. Jiang et al.  demonstrated an improved approach of free surface electrospinning utilizing micro-bubble solu-tion system and studied the effect of bubble size on the diameters of nanofibers. Figure 1 shows different nanofiber morphologies of different polymer via bubble electrospinning.
(a) (b) (c)
(d) (e) (f) Figure 1. The scanning electron microscopy of the nanofiber membrane via bubble spinning set-ups; (a) PVA (DI water) nanofiber, (b) PES (DMF) nanofiber, (c) PLA(DMF) nanofiber, (d) PES (DMF) nanopore fibers; (e) nylon (formic acid) nanofibers; (f) PS(THF) nanofibers
These researches mainly focused on the preparation and application of various poly-mer nanofibers via bubble electrospinning, but fewer literature reported the dynamical mecha-nism of bubble forming and its application in electro-spinning for mass production of nanofibers. In view of this, in this paper, the growth situation and rupture process of un-charged and charged polymer bubble were discussed, which further explained the reasons why bubble electrospinning will be one of the most effective methods for mass production of nanofiber.
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149 1143
Materials: PVA, with an average molecular weight of 95,000 g/mol purchased from Aladdin, sodium dodecyl benzene sulfonate (SDBS) purchased from Sinopharm Chemical Reagent Co., Ltd, and deionized water were used in these experiments. All materials used without further purification.
Solution preparation: PVA particles and SDBS powder were dissolved into DI water at the room temperature. The mixture was then placed on a 120 °C heating plate and stirred until a homogeneous and transparent solution was obtained. The solution was then cooled down to room temperature for experiment. The concentration of PVA solution was 6 wt.%.
Electrospinning set-up: fig. 2 shows the schematic of a classical bubble spinning set-up, which includes a bubble generator, a spinneret, an air pump, a solution reservoir, a high-voltage pow-er supply, and a grounded collector. The grounded collector was placed 20 cm upper to the spinneret.
The forming and vanishing process of un-charged and charged polymer bubbles were respec-tively recorded with a high speed camera (HSC). The photos were further dissected to investigate the growth and rupture process of bubble.
During the experimental process, to begin with, the air pump was switched on until the gen-erated bubbles were continuously pumped into the spinneret; the growth and rupture process of the un-charged bubble was videoed. And then, the ap-plied voltage was applied and increased until a number of jets were observed from the top of the spinneret, the movement of the charged bubbles was also videoed. The experiments were carried out at room temperature in the air.
Shown as fig. 1, nanofibres with various morphologies, such as smooth, nanoporous, micro-spherical with nanoporous, can be fabricated. The key to a successful bubble electrosping is the steady continuous generation and rupture of polymer bubbles.
The nanofiber formation and the obtained nanofiber properties in bubble electrospinning depend on polymer solution properties including viscosity, solution concen-tration, surface tension and electrical conductivity.
Young-Laplace equation When an air bubble generates from the surface of a polymer solution, the force
pushing it upward can be expressed in the form:
2upward in out( )πF P P R= − (1)
where Pin is the inner pressure of the bubble，Pout – the out pressure of the bubble, and R – the radius of the bubble. The gravitation could be ignored as the mass of bubble is extremely low.
The downward force of bubble, related with the surface tension of polymer solution, can be expressed in the form:
Figure 2. The schematic of a classical bubble spinning set-up
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning 1144 THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149
downward 2πF Rγ= (2)
where γ is the surface tension of polymer solution. Since
upward downwardF F= (3)
it`s surface tension T can be expressed in the form :
in out1 ( )2
T R P P= − (4)
When the bubble has an aspheric surface, the inner radius of the bubble can be ex-pressed as R1 and R2, according to the Laplace equation, it`s surface tension T can be also ex-pressed in the form:
1 1P P
According to eqs. (4) and (5), we can see that the surface tension is related with the di-ameter of the bubble and the inner and outside pressure difference on the bubble, but not with whatever the polymer is. Therefore, as long as a solution can form bubbles, these equations can be used to guide the fabrication nanofibers in bubble electrospinning. What`s more, the pres-sure difference of bubble between inside and outside is the most important parameter which has effects on the rupture of polymer bubble (fig. 3).
Unstable growth of bubble
HSC was used to record the growth pro-cess of polymer bubbles. Figure 4 shows the
photos of growth process. To quantify this process, the height, width and angel of the bubble were measured per 10 ms and the methods of measurement were shown as figs. 5(a) and (b). The height, width and angel of the bubble were always changing during the growth process, figs. 5(a) and (b) show the increasing tendency of the height, width and angel.
The longitudinal and transverse growth rates in per 10ms can be calculated by
Vl = dj – di (6)
Vt = dn – dm (7)
where Vl and Vt are the longitudinal and transverse growth rates per 10 ms, dj – di and dn – dm are the difference of height and width per 10 ms.
Shown as figs. 5(c) and (d), Vl and Vt vary greatly during the whole growth process. Sometimes they get bigger, sometimes they get smaller. After about 300 ms, they even drop
Figure 3. The force analysis model of bubble
hen, R., et al.: BHERMAL SCIEN
elow zero whe difference bon become mrocess of bubupture processhich makes tubble electroshich is very a
Figurere many polade a rough any jets were
That ie unstable and
upture of pol
Whenubble vanisheg polymer bu
Bubble Rupture NCE, Year 2015
Figure 4. Hig
hich means thbetween adja
more and mobble was extres. As we all the polymer spinning, theadvantageous
nt and morph
re 6 shows thalymer solutiobubble surfa
e produced onis to say, durid rough polym
n a bubble ones. But this isubble, which
in Bubble Electr5, Vol. 19, No. 4
gh speed photo
he size of bubacent peak anre unstable. emely unstabknow, more surface unst
e unstable surs for generatin
hology of po
at the polymeon ripples andace. In this can the rough poing the growtmer bubble su
n a liquid-gass not what hapwere videoed
rospinning 4, pp. 1141-1149
ography of poly
bble is smalled valley poinAll descripte
ble, especiallyTylor corns
table more earface is ingenng more Tylo
er solution flod tiny bubblesase, Taylor-lolymer surfacth process, theurface; the spi
s interface rupppened. Figud by HSC at 2
ymer bubble g
er than the sint greaten, whed phenomeny in the verycan be generasily in neednerate during
or cones at the
owed fast alons, caused by tike cones coce if a voltage nanofibers cinning proces
ptures, the geure 8 is a coll2000 frames p
ze last 10 mshich means thna indicated t
short time-frrated under adle-less electrg the whole ge same voltag
ng the bubblethe incoming
ould be easilye was appliedcan be easily ss was shown
eneral expectection of phoper second. I
s. What`s mohe growth situthat the growrame before ta higher voltarospinning. Fgrowth procege.
e surface. Theg airflow, whiy generated ad. fabricated froas fig. 7.
tation is that totos of a ruptt shows that t
ore, ua-wth the age For ess,
ere ich and
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning 1146 THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149
polymer bubble ruptures into many smaller thin films and tiny droplets. Therefore, the rup-tured thin film is more precisely expected to retract rapidly until it becomes part of the inter-face, which typically occurs within milliseconds.
(c) (d) Figure 5. The changes during the growth of polymer bubble; (a) the changing of the bubble high and width, (b) the changing of the bubble angel, (c) longitudinal growth rate, and (d) transverse growth rate
As we all know, during the industrialization process of nanofiber production, one of the most profound difficulties is how to increase the number of Tylor cones, and many re-searchers explored lots of methods to improve it, the typically one was increasing the number of needles. However, for the bubble spinning, this problem can be solved considerably easier,
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149 1147
because a bubble ruptures into hundreds of tiny thin films and droplets which are the Tylor cones for fabricating mass nanofibers.
Figure 6. The movement and morphology of polymer bubble film
Figure 7. The electrospinning before the bubble rupture
Figure 8. The rupture of polymer bubble
Figure 9 shows the rupture process of charged polymer bubble, which was videoed by HSC at 500 frames per second. Lots of jets go up to the ground collector after the charged polymer bubble rupture, which typically occurs within milliseconds. All these jets are formed from these tiny droplets and shredded bubble films. Figure 10 shows the bubble electrospinning process, which was taken by digital single lens reflex camera. Thousands of polymer jets, looks like a waterfall, are spraying toward the ground collector after applying high-voltage direct-current power. The production of PVA nanofibers are about 3 g/hour via single bubble electrospinning.
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning 1148 THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149
(a) (b) (c) (d)
Figure 9. The rupture of charged polymer bubble, videoed by HSC
The paper reported the dynamics mechanism of polymer bubble and its application in electro-spinning for mass production of nanofibers. According to the Yang- -Laplace equation, the surface tensile of bubble is only related with the diameter and pressure difference of bub-ble between inside and outside. Therefore, the growth and rupture of bubble can be controlled by changing the in-side pressure of bubble, which affect the stability, conti-nuity, efficiency of bubble electrospinning. Based on high speed photos, the dynamic mechanism, including growth, and rupture process, of polymer bubble was investigated. The unstable growth situation of bubble made the
electrospinning more easily under a lower voltage; Tylor cones could be easily generated and many jets were produced on the rough polymer bubble surface after applying a voltage. What is more, thousands of tiny droplets and shredded bubble films, which were generated from the ruptured bubbles, were Taylor-like cones for producing polymer jets and fabricating mass nanofibers.
In conclusion, bubble electrospinning has some innate advantages in electrospinning. It definitely is one of the most effective methods for mass production of nanofibers and its set-up also deserves further exploration on the improvement and optimiz-ing.
The work is supported financially by PAPD (A Project Funded by the Priority Aca-demic Program Development of Jiangsu Higher Education Institutions), Natural Science Foundation of the Jiangsu Higher Education Institutions of China (Grant No. 12KJB130002), National Natural Science Foundation of China under Grant Nos. 10802021 and 10972053, and Nantong Textile Institute of Soochow University, Academic new artist doctoral post graduate of Soochow University.
 Reneker, D. H., Chun, I., Nanometre Diameter Fibres of Polymer, Produced by Electrospinning, Nano-technology, 7 (1996), 3, pp. 216-223
 Fujihara, K., et al., An Introduction to Electrospinning and Nanofibers, World Scientific, Singapore, 2005
Figure 10. The bubble spinning for mass production
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149 1149
 Wang, X., et al., Needleless Electrospinning of Uniform Nanofibers Using Spiral Coil Spinnerets, Jour-nal of Nanomaterials, 2012 (2012), ID 785920
 Petrik, S., Maly, M., Production Nozzle-Less Electrospinning Nanofiber Technology, Proceedings, MRS 1240 (2009), DOI: http://dx.doi.org/10.1557/PROC-1240-WW03-07
 Chen, R. X., et al., Bubbfil Spinning for Mass-Production of Nanofibers, Thermal Science, 18 (2014), 5, pp. 1718-1719
 Liu, Y, He, J.-H., Bubble Electrospinning for Mass Production of Nanofibers. International Journal of Nonlinear Sciences and Numerical Simulation, 8 (2007), 3, pp. 393-396
 Liu, Y, et al., Bubble-Electrospinning: A Novel Method for Making Nanofibers, Proceedings, 2007 In-ternational Symposium on Nonlinear Dynamics, Pts 1-4. Vol. 96. Ed. J.-H. He; 2008: Journal of Physics Conference Series
 He, J.-H., The Smaller, the Better: From the Spider-Spinning to Bubble-Electrospinning, Acta Physica Polonica A, 121 (2012), 1, pp. 254-256
 Liu, Y., et al., The Principle of Bubble Electrospinning and Its Experimental Verification, Journal of Polymer Engineering, 28 (2008), 1-2, pp. 55-65
 Yang, R. R., et al., Effect of Solution Concentration on Diameter and Morphology of PVA Nanofibres in Bubble Electrospinning Process, Materials Science and Technology, 26 (2010), 11, pp. 1313-1316
 Kong, H.-Y., et al., Polymer Liquid Membrane for Nanofiber Fabrication, Thermal Science, 17 (2013), 5, pp. 1479-1482
 Gule, N. P., et al., Furanone-Containing Poly (Vinyl Alcohol) Nanofibers for Cell-Adhesion Inhibition, Water Research, 47 (2013), 3, pp. 1049-1059
 Dou, H., et al., Effect of Solution Concentrations on the Morphology of Nylon6/66 Nanofibrous Yarns by Blown Bubble-Spinning, Materia, 19 (2014), 4, pp. 358-362
 Chen, R.-X., et al., Mechanism of Nanofiber Crimp, Thermal Science, 17 (2013), 5, pp. 1473-1477  Chen. R.-X., On Surface Tension of a Bubble under Presence of Electrostatic Force, Thermal Science,
19 (2015), 1, pp. 353-355  Li, Z.-B., et al., On Air Blowing Direction in the Blown Bubble-Spinning, Materia, 19 (2014), 4, pp.
345-349  Li, Y., et al., Comparison between Electrospun and Bubbfil-Spun Polyether Sulfone Fibers, Materia, 19
(2014), 4, pp. 363-369  Shen, J., et al., Bio-Mimic Design of PM2.5 Anti-Smog Masks, Thermal Science, 18 (2014), 5, pp.
1689-1690  Sidaravicius, J., et al., The Influence of Solution Parameters on the Electrospinning Intensity from
Foamed Surface, Journal of Applied Polymer Science, 132 (2015), 23, pp. 42034-42041  Ren, X., et al., Foaming-Assisted Electrospinning of Large-Pore Mesoporous ZnO Nanofibers with Tai-
lored Structures and Enhanced Photocatalytic Activity, RSC Advances, 5 (2015), 21, pp. 16361-16367  Jiang, G., et al. An Improved Free Surface Electrospinning with Micro-Bubble Solution System for
Massive Production of Nanofibers, Materials Letters, 144 (2015), 4, pp. 22-25
Paper submitted: January 28, 2015 Paper revised: May 18, 2015 Paper accepted: May 26, 2015